# A Crystal Plasticity FE Analysis Considering The phase transformation of the former, alter the...

date post

24-Aug-2020Category

## Documents

view

0download

0

Embed Size (px)

### Transcript of A Crystal Plasticity FE Analysis Considering The phase transformation of the former, alter the...

[溶接学会論文集 第 33 巻 第 ○ 号 p. 000s-000s（2015)]

A Crystal Plasticity FE Analysis Considering Mechanically Induced Martensitic Phase Transformation

by Seiichiro Tsutsumi**, Riccardo Fincato**, Kazushi Ueda*** and Kenjiro Terada****

One of the most challenging topic nowadays for the steel manufacturers is the investigation of the role of the retained austenitic grains inside a martensitic body. The phase transformation of the former, in fact, has been proved to alter the material properties in terms of toughness, ductility, resistance and also it has be indicated as one of the probable causes for the crack initiation. The work presented in this paper aims to study this phenomena by means of a thermodynamically based single crystal constitutive model, coupling the crystallographic slip together with the phase transformation.

Key Words: Crystal Plasticity, Martensitic Phase Transformation, Retain Austenite, FE analyses.

1. Introduction

Depending on the carbon content of the austenite, the martensite start temperature (Ms) and the finish one (Mf) can be sensibly altered. In particular, for a high level of carbon, the previous two temperatures are depressed, leading to difficulties in converting all of the austenite to martensite. When this condition is satisfied it is possible to have retained austenite, which may be either extremely non-desirable or desirable depending on the nature of the steel component and on its operative use.

It is also important to know the percentage and the distribution of the retain austenite since the transformation from metastable austenitic phase to martensitic phase has been considered to change the material response1), but more importantly, to decrease the fracture toughness of materials2). It has, in fact, been proved that they can have an effect on the local stress and strain distributions through the elongation and volume change during the martensitic phase transformation, accompanied with the lattice-invariant shear.

In this study, local stress distribution at a crystal level has been analyzed by means of FE numerical simulations adopting the crystal plasticity theory and the mechanically induced martensitic transformation (MIMT) under a thermodynamically based single crystal constitutive model. The kinetics of the transformation, in terms of the definition of the orientation of the relationship between the parent austenitic and the martensitic variants, is modeled by taking into consideration the well-known

Kurdjumov–Sachs (KS) relationship. The effect of mechanically induced martensitic transformation on the local stress distribution is discussed under uniaxial extension condition.

2. Constitutive model

One of the principal variables to consider when dealing with the finite strain theory is the deformation gradient, which creates a map (see Fig. 1) between the points coordinates of the deformed (current) configuration and the ones of the undeformed (reference).

Fig. 1 Multiplicative decomposition of the deformation gradient.

The constitutive model adopted in the present study consider a multiplicative decomposition of the total deformation gradient

into three parts: an elastic one eF (which describes the distortion of the crystal lattice), the deformation caused by the

austenite-martensitic transformation process tF and finally the irreversible plastic slip on the crystallographic planes pF :

e t pF F F F (1)

The position of the transformation term can vary depending on the different authors’ approach, in this paper we adopted the one proposed by Idesman et al.3) and extended by the authors4). The crystallographic slip can take place whenever the

resolved shear stress on a slip surface ( ) assumes a value greater

*Received: 2014.11.28 **Member, Joining and Welding Research Institute, Osaka

University. ***Student Member, Joining and Welding Research Institute,

Osaka University. ****International Research Institute of Disaster Science

(IRIDeS), Tohoku University.

［溶接学会論文集 第 33 巻 第 2 号 p. 102s-106s （2015）］

2 研究論文 □他：□□□□□□□□□□□□□□□□□□□□□□□□□□□□□□□□□□□

than the critical one, commonly named CRSS. The reference framework for the crystal plasticity constitutive theory is the one presented by Asaro and Lubarda5) and by Pierce, Asaro and Needleman6), 7). They expressed the CRSS by means of the unit

vector defining the slip directions *( )s , the one normal to the sliding plane *( )m (the subscript 0 indicates the reference configuration) and the Kirchhoff stress Jσ as shown in as in Eq.(2):

*( ) ( ) *( ) ( ) 1 1

0 0

( ) *( ) *( )

; ;

:

e t t e

J

s F F s m m F F

s m σ (2)

The total plastic work can be imagined as formed by the sum of the plastic works of each slip system, allowing to write:

( ) ( ) *( ) *( ) ( ) 1 1

: ; n n

p pJ

σ l l s m (3) pl is the plastic velocity deformation gradient (obtainable by

taking the time derivative of Eq. (1)) and ( ) is the crystallographic slip, assumed in accordance with8):

( ) ( ) ( ) ( ) ( ) ( ) ( )

1

2 0 0 0

; ;

sech ;

v nn

s

a g sign g g h

h h h h qh

(4)

a is the reference slip system, ( )g is the slip resistance of the system, nv controls the strain rate dependency and h is the hardening moduli.

As it was implicitly done for the crystal plasticity, it is also possible to assume that the phase transformation happens at a material point, where the total transformation deformation

gradient, tF in Eq.(1), can be thought as a linear combination of special deformation gradients, each of them associated with a geometrical pattern proper of the material variants, and coefficients c, which give the measure on how predominant is a variant respect to the others:

( ) ( ) 0

ˆ m

t t p p

p c

F F (5)

the index p, from 1 to m, represents the different variants, whereas the p=0 case defines the matrix.

The formulation of these ( ) ( , )pc tx multipliers passes through the Clausius-Duhem inequality for the definition of a functional form from which it is possible to derive the exact mathematical expression. These coefficients can be physically interpreted as multiplier of the matrix and variants fractions each of which expressing a different deformation pattern ( )ˆ t pF . In different words they represent a fraction of a unitary volume associated with a specific deformation mechanisms proper of the crystallographic structure of the material, otherwise called variants9), 10). For a more complete description of the variables the reader is referred to11).

It is worth mentioning that the numerical model is provided with a sort of activation energy; if the module of the thermodynamic driving force assumes a value bigger that this energetic threshold the transformation from the matrix to the variants, or from one variant to another, can take place. This aspect is quite relevant since it guarantees a stable state for the austenitic phase, which otherwise could transform under every conditions.

The expression of the Cauchy stress rate in the current configuration derived from the hypo-elasticity framework developed by the reference 5).

3. Numerical models

The purpose of this paper is to describe the behavior of the retained austenite transformation inside a martensitic body in order to better understand the effect of this mechanism in terms of stress/strain distribution and localization. In the following paragraphs two different numerical examples have been carried out to investigate the role of the shape of the inclusion and the crystal plasticity influence during the phase transformation. All the simulations have been realized by means of a user subroutine inside the commercial finite element code Abaqus v6.13-1412).

3.1 Shape effect of the austenitic grain

The first numerical example deals with the investigation of the shape effect of a retained austenite grain surrounded by an elastic martensitic body. Figure 2 displays the mesh used in the computation (C3D8R brick elements) and the boundary conditions adopted. The alignment of the transformable material, which dimensions are L/3xL/3 in the squared case (i.e. CASE A) and r=L/6 in the rounded one (i.e. CASE B), is placed in the center of the sample and surrounded by a purely linear elastic body. The mechanical properties have been assumed accordingly to Yoshida et al.’s previous work4).

Forced displacement (3D plane strain)

L

L

L/3

L/3

material T (transformable)

material E (elastic)

ＡＢ

Ｃ Ｃ’

Ａ’Ｂ’

O

a) b)

Fig. 2 (a) CASE A squared inclusion, (b) CASE B rounded inclusion.

103s溶 接 学 会 論 文 集 第 33 巻（2015）第 2号

*View more*